# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_nb-448r-5

_audit_creation_date             2013-12-30T15:21:24-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'

#==============================================================================

# CHEMICAL DATA

_chemical_name_systematic        
;
 ?
;
_chemical_formula_sum            'Cr0.50 Li2 O3 Sb0.50'
_chemical_formula_weight         148.76

#==============================================================================

# CRYSTAL DATA

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   5.1368(12)
_cell_length_b                   8.890(2)
_cell_length_c                   9.809(3)
_cell_angle_alpha                90
_cell_angle_beta                 99.93(2)
_cell_angle_gamma                90
_cell_volume                     441.22(19)
_cell_formula_units_Z            8
_cell_measurement_temperature    293(2)
_exptl_crystal_density_diffrn    4.479
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             540
_exptl_absorpt_coefficient_mu    8.526
_exptl_absorpt_correction_type   none

#==============================================================================

# EXPERIMENTAL DATA

_exptl_special_details           
;
 ?
;
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  graphite
_diffrn_reflns_number            2930
_diffrn_reflns_av_R_equivalents  0.0487
_diffrn_reflns_av_unetI/netI     0.0345
_diffrn_reflns_theta_min         4.22
_diffrn_reflns_theta_max         28.88
_diffrn_reflns_theta_full        28.88
_diffrn_measured_fraction_theta_max 0.944
_diffrn_measured_fraction_theta_full 0.944
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_limit_l_max       13

#==============================================================================

# STRUCTURE SOLUTION

_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom

#==============================================================================

# REFINEMENT DATA

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;
_reflns_number_total             544
_reflns_number_gt                508
_reflns_threshold_expression     >2sigma(I)
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_R_factor_all          0.0516
_refine_ls_R_factor_gt           0.0456
_refine_ls_wR_factor_ref         0.1139
_refine_ls_goodness_of_fit_ref   1.255
_refine_ls_restrained_S_all      1.255
_refine_ls_number_reflns         544
_refine_ls_number_parameters     44
_refine_ls_number_restraints     0
_refine_ls_hydrogen_treatment    mixed
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0522P)²+2.1214P] where P=(Fo²+2Fc²)/3'
_refine_ls_shift/su_max          0
_refine_ls_shift/su_mean         0
_refine_diff_density_max         1.534
_refine_diff_density_min         -0.929
_refine_diff_density_rms         0.304
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.0022(7)
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'

#==============================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_type_symbol
Li1 0.245(2) 0.0785(13) 0.0004(10) 0.020(3) Uani d . 1 . . Li
Li2 0.25 0.25 0.5 0.023(4) Uani d S 1 . . Li
Sb1 0 0.75128(7) 0.25 0.0061(3) Uani d SP 0.75 . . Sb
Li3 0 0.75128(7) 0.25 0.0061(3) Uani d SP 0.25 . . Li
Li4 0 0.0869(4) 0.25 0.0254(8) Uani d SP 0.47 . . Li
Cr1 0 0.0869(4) 0.25 0.0254(8) Uani d SP 0.53 . . Cr
Cr2 0 0.41940(12) 0.25 0.0029(4) Uani d SP 0.45 . . Cr
Li5 0 0.41940(12) 0.25 0.0029(4) Uani d SP 0.3 . . Li
Sb5 0 0.41940(12) 0.25 0.0029(4) Uani d SP 0.25 . . Sb
O1 0.1380(10) 0.2546(5) 0.1363(5) 0.0137(11) Uiso d . 1 . . O
O2 0.1175(10) 0.5876(5) 0.1360(5) 0.0129(11) Uiso d . 1 . . O
O3 0.1288(10) 0.9106(5) 0.1347(5) 0.0139(11) Uiso d . 1 . . O



#==============================================================================

# MOLECULAR GEOMETRY

_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Li1 O3 5_565 2.137(11) ?
Li1 O2 3_545 2.138(11) ?
Li1 O3 1_545 2.142(11) ?
Li1 O1 7 2.154(11) ?
Li1 O1 . 2.186(12) ?
Li1 O2 7 2.191(12) ?
Li1 Li1 5 2.87(2) ?
Li1 Li2 4_545 2.921(12) ?
Li1 Sb5 3_545 2.935(10) ?
Li1 Li5 3_545 2.935(10) ?
Li1 Cr2 3_545 2.935(10) ?
Li1 Li4 . 2.939(10) ?
Li2 O3 6_566 2.111(5) ?
Li2 O3 4_545 2.111(5) ?
Li2 O2 6_566 2.154(5) ?
Li2 O2 4_545 2.154(5) ?
Li2 O1 8_556 2.201(5) ?
Li2 O1 2 2.201(5) ?
Li2 Li1 6_556 2.921(12) ?
Li2 Li1 4 2.921(12) ?
Li2 Li4 . 2.9458(17) ?
Li2 Cr1 7_556 2.9458(17) ?
Li2 Li4 7_556 2.9458(17) ?
Sb1 O2 2 1.991(5) ?
Sb1 O2 . 1.991(5) ?
Sb1 O3 . 1.996(5) ?
Sb1 O3 2 1.996(5) ?
Sb1 O1 4 1.997(5) ?
Sb1 O1 3_455 1.997(5) ?
Sb1 Cr2 . 2.9504(14) ?
Sb1 Cr1 3_455 2.9549(17) ?
Sb1 Li4 3_455 2.9549(17) ?
Sb1 Cr1 3 2.9549(17) ?
Li4 O1 2 2.060(5) ?
Li4 O1 . 2.060(5) ?
Li4 O2 4_545 2.086(5) ?
Li4 O2 3_445 2.086(5) ?
Li4 O3 1_545 2.105(5) ?
Li4 O3 2_545 2.105(5) ?
Li4 Li1 2 2.939(10) ?
Li4 Li2 2 2.9458(17) ?
Li4 Li1 5 2.951(10) ?
Li4 Li1 6_556 2.951(10) ?
Cr2 O2 . 2.020(5) ?
Cr2 O2 2 2.020(5) ?
Cr2 O1 . 2.041(5) ?
Cr2 O1 2 2.041(5) ?
Cr2 O3 3_445 2.044(5) ?
Cr2 O3 4_545 2.044(5) ?
Cr2 Li1 4 2.935(10) ?
Cr2 Li1 3_455 2.935(10) ?
O1 Li3 3_545 1.997(5) ?
O1 Sb1 3_545 1.997(5) ?
O1 Li1 7 2.154(11) ?
O1 Li2 2 2.201(5) ?
O2 Cr1 3 2.086(5) ?
O2 Li4 3 2.086(5) ?
O2 Li1 3_455 2.138(11) ?
O2 Li2 4 2.154(5) ?
O2 Li1 7 2.191(12) ?
O3 Sb5 3 2.044(5) ?
O3 Li5 3 2.044(5) ?
O3 Cr2 3 2.044(5) ?
O3 Cr1 1_565 2.105(5) ?
O3 Li4 1_565 2.105(5) ?
O3 Li2 4 2.111(5) ?
O3 Li1 5_565 2.137(11) ?
O3 Li1 1_565 2.142(11) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Li1 O2 175.3(6) 5_565 3_545 ?
O3 Li1 O3 95.6(5) 5_565 1_545 ?
O2 Li1 O3 87.5(4) 3_545 1_545 ?
O3 Li1 O1 84.3(4) 5_565 7 ?
O2 Li1 O1 92.5(4) 3_545 7 ?
O3 Li1 O1 179.3(6) 1_545 7 ?
O3 Li1 O1 93.1(5) 5_565 . ?
O2 Li1 O1 83.4(4) 3_545 . ?
O3 Li1 O1 89.9(4) 1_545 . ?
O1 Li1 O1 90.7(5) 7 . ?
O3 Li1 O2 90.1(4) 5_565 7 ?
O2 Li1 O2 93.2(5) 3_545 7 ?
O3 Li1 O2 93.4(5) 1_545 7 ?
O1 Li1 O2 86.0(4) 7 7 ?
O1 Li1 O2 175.1(6) . 7 ?
O3 Li1 Li1 47.9(3) 5_565 5 ?
O2 Li1 Li1 135.2(6) 3_545 5 ?
O3 Li1 Li1 47.7(3) 1_545 5 ?
O1 Li1 Li1 132.2(6) 7 5 ?
O1 Li1 Li1 92.2(5) . 5 ?
O2 Li1 Li1 92.6(6) 7 5 ?
O3 Li1 Li2 93.0(4) 5_565 4_545 ?
O2 Li1 Li2 91.8(4) 3_545 4_545 ?
O3 Li1 Li2 46.2(3) 1_545 4_545 ?
O1 Li1 Li2 133.2(5) 7 4_545 ?
O1 Li1 Li2 136.1(4) . 4_545 ?
O2 Li1 Li2 47.2(3) 7 4_545 ?
Li1 Li1 Li2 61.5(4) 5 4_545 ?
O3 Li1 Sb5 139.8(5) 5_565 3_545 ?
O2 Li1 Sb5 43.5(2) 3_545 3_545 ?
O3 Li1 Sb5 44.1(2) 1_545 3_545 ?
O1 Li1 Sb5 135.9(5) 7 3_545 ?
O1 Li1 Sb5 87.7(3) . 3_545 ?
O2 Li1 Sb5 92.3(4) 7 3_545 ?
Li1 Li1 Sb5 91.9(5) 5 3_545 ?
Li2 Li1 Sb5 61.0(2) 4_545 3_545 ?
O3 Li1 Li5 139.8(5) 5_565 3_545 ?
O2 Li1 Li5 43.5(2) 3_545 3_545 ?
O3 Li1 Li5 44.1(2) 1_545 3_545 ?
O1 Li1 Li5 135.9(5) 7 3_545 ?
O1 Li1 Li5 87.7(3) . 3_545 ?
O2 Li1 Li5 92.3(4) 7 3_545 ?
Li1 Li1 Li5 91.9(5) 5 3_545 ?
Li2 Li1 Li5 61.0(2) 4_545 3_545 ?
Sb5 Li1 Li5 0.00(4) 3_545 3_545 ?
O3 Li1 Cr2 139.8(5) 5_565 3_545 ?
O2 Li1 Cr2 43.5(2) 3_545 3_545 ?
O3 Li1 Cr2 44.1(2) 1_545 3_545 ?
O1 Li1 Cr2 135.9(5) 7 3_545 ?
O1 Li1 Cr2 87.7(3) . 3_545 ?
O2 Li1 Cr2 92.3(4) 7 3_545 ?
Li1 Li1 Cr2 91.9(5) 5 3_545 ?
Li2 Li1 Cr2 61.0(2) 4_545 3_545 ?
Sb5 Li1 Cr2 0.00(4) 3_545 3_545 ?
Li5 Li1 Cr2 0.00(4) 3_545 3_545 ?
O3 Li1 Li4 92.8(4) 5_565 . ?
O2 Li1 Li4 86.9(3) 3_545 . ?
O3 Li1 Li4 45.7(2) 1_545 . ?
O1 Li1 Li4 135.0(5) 7 . ?
O1 Li1 Li4 44.4(2) . . ?
O2 Li1 Li4 139.1(5) 7 . ?
Li1 Li1 Li4 61.0(3) 5 . ?
Li2 Li1 Li4 91.8(3) 4_545 . ?
Sb5 Li1 Li4 60.72(19) 3_545 . ?
Li5 Li1 Li4 60.72(19) 3_545 . ?
Cr2 Li1 Li4 60.72(19) 3_545 . ?
O3 Li2 O3 180.0000(10) 6_566 4_545 ?
O3 Li2 O2 84.7(2) 6_566 6_566 ?
O3 Li2 O2 95.3(2) 4_545 6_566 ?
O3 Li2 O2 95.3(2) 6_566 4_545 ?
O3 Li2 O2 84.7(2) 4_545 4_545 ?
O2 Li2 O2 180.0000(10) 6_566 4_545 ?
O3 Li2 O1 86.63(19) 6_566 8_556 ?
O3 Li2 O1 93.37(19) 4_545 8_556 ?
O2 Li2 O1 89.21(19) 6_566 8_556 ?
O2 Li2 O1 90.79(19) 4_545 8_556 ?
O3 Li2 O1 93.37(19) 6_566 2 ?
O3 Li2 O1 86.63(19) 4_545 2 ?
O2 Li2 O1 90.79(19) 6_566 2 ?
O2 Li2 O1 89.21(19) 4_545 2 ?
O1 Li2 O1 180 8_556 2 ?
O3 Li2 Li1 47.1(2) 6_566 6_556 ?
O3 Li2 Li1 132.9(2) 4_545 6_556 ?
O2 Li2 Li1 131.7(2) 6_566 6_556 ?
O2 Li2 Li1 48.3(2) 4_545 6_556 ?
O1 Li2 Li1 89.3(2) 8_556 6_556 ?
O1 Li2 Li1 90.7(2) 2 6_556 ?
O3 Li2 Li1 132.9(2) 6_566 4 ?
O3 Li2 Li1 47.1(2) 4_545 4 ?
O2 Li2 Li1 48.3(2) 6_566 4 ?
O2 Li2 Li1 131.7(2) 4_545 4 ?
O1 Li2 Li1 90.7(2) 8_556 4 ?
O1 Li2 Li1 89.3(2) 2 4 ?
Li1 Li2 Li1 180.0(4) 6_556 4 ?
O3 Li2 Li4 93.14(14) 6_566 . ?
O3 Li2 Li4 86.86(14) 4_545 . ?
O2 Li2 Li4 134.94(14) 6_566 . ?
O2 Li2 Li4 45.06(14) 4_545 . ?
O1 Li2 Li4 135.69(13) 8_556 . ?
O1 Li2 Li4 44.31(13) 2 . ?
Li1 Li2 Li4 60.4(2) 6_556 . ?
Li1 Li2 Li4 119.6(2) 4 . ?
O3 Li2 Cr1 86.86(14) 6_566 7_556 ?
O3 Li2 Cr1 93.14(14) 4_545 7_556 ?
O2 Li2 Cr1 45.06(14) 6_566 7_556 ?
O2 Li2 Cr1 134.94(14) 4_545 7_556 ?
O1 Li2 Cr1 44.31(13) 8_556 7_556 ?
O1 Li2 Cr1 135.69(13) 2 7_556 ?
Li1 Li2 Cr1 119.6(2) 6_556 7_556 ?
Li1 Li2 Cr1 60.4(2) 4 7_556 ?
Li4 Li2 Cr1 180 . 7_556 ?
O3 Li2 Li4 86.86(14) 6_566 7_556 ?
O3 Li2 Li4 93.14(14) 4_545 7_556 ?
O2 Li2 Li4 45.06(14) 6_566 7_556 ?
O2 Li2 Li4 134.94(14) 4_545 7_556 ?
O1 Li2 Li4 44.31(13) 8_556 7_556 ?
O1 Li2 Li4 135.69(13) 2 7_556 ?
Li1 Li2 Li4 119.6(2) 6_556 7_556 ?
Li1 Li2 Li4 60.4(2) 4 7_556 ?
Li4 Li2 Li4 180 . 7_556 ?
Cr1 Li2 Li4 0 7_556 7_556 ?
O2 Sb1 O2 86.1(3) 2 . ?
O2 Sb1 O3 177.91(16) 2 . ?
O2 Sb1 O3 92.2(2) . . ?
O2 Sb1 O3 92.2(2) 2 2 ?
O2 Sb1 O3 177.91(16) . 2 ?
O3 Sb1 O3 89.5(3) . 2 ?
O2 Sb1 O1 92.3(2) 2 4 ?
O2 Sb1 O1 88.9(2) . 4 ?
O3 Sb1 O1 86.5(2) . 4 ?
O3 Sb1 O1 92.3(2) 2 4 ?
O2 Sb1 O1 88.9(2) 2 3_455 ?
O2 Sb1 O1 92.3(2) . 3_455 ?
O3 Sb1 O1 92.3(2) . 3_455 ?
O3 Sb1 O1 86.5(2) 2 3_455 ?
O1 Sb1 O1 178.3(2) 4 3_455 ?
O2 Sb1 Cr2 43.04(13) 2 . ?
O2 Sb1 Cr2 43.04(13) . . ?
O3 Sb1 Cr2 135.23(14) . . ?
O3 Sb1 Cr2 135.23(14) 2 . ?
O1 Sb1 Cr2 90.86(12) 4 . ?
O1 Sb1 Cr2 90.86(12) 3_455 . ?
O2 Sb1 Cr1 44.84(15) 2 3_455 ?
O2 Sb1 Cr1 89.21(15) . 3_455 ?
O3 Sb1 Cr1 136.40(15) . 3_455 ?
O3 Sb1 Cr1 88.73(15) 2 3_455 ?
O1 Sb1 Cr1 137.14(14) 4 3_455 ?
O1 Sb1 Cr1 44.09(14) 3_455 3_455 ?
Cr2 Sb1 Cr1 60.37(5) . 3_455 ?
O2 Sb1 Li4 44.84(15) 2 3_455 ?
O2 Sb1 Li4 89.21(15) . 3_455 ?
O3 Sb1 Li4 136.40(15) . 3_455 ?
O3 Sb1 Li4 88.73(15) 2 3_455 ?
O1 Sb1 Li4 137.14(14) 4 3_455 ?
O1 Sb1 Li4 44.09(14) 3_455 3_455 ?
Cr2 Sb1 Li4 60.37(5) . 3_455 ?
Cr1 Sb1 Li4 0 3_455 3_455 ?
O2 Sb1 Cr1 89.21(15) 2 3 ?
O2 Sb1 Cr1 44.84(15) . 3 ?
O3 Sb1 Cr1 88.73(15) . 3 ?
O3 Sb1 Cr1 136.40(15) 2 3 ?
O1 Sb1 Cr1 44.09(14) 4 3 ?
O1 Sb1 Cr1 137.14(14) 3_455 3 ?
Cr2 Sb1 Cr1 60.37(5) . 3 ?
Cr1 Sb1 Cr1 120.73(11) 3_455 3 ?
Li4 Sb1 Cr1 120.73(11) 3_455 3 ?
O1 Li4 O1 87.3(3) 2 . ?
O1 Li4 O2 95.1(2) 2 4_545 ?
O1 Li4 O2 84.7(2) . 4_545 ?
O1 Li4 O2 84.7(2) 2 3_445 ?
O1 Li4 O2 95.1(2) . 3_445 ?
O2 Li4 O2 179.7(3) 4_545 3_445 ?
O1 Li4 O3 177.87(18) 2 1_545 ?
O1 Li4 O3 94.5(2) . 1_545 ?
O2 Li4 O3 86.3(2) 4_545 1_545 ?
O2 Li4 O3 93.9(2) 3_445 1_545 ?
O1 Li4 O3 94.5(2) 2 2_545 ?
O1 Li4 O3 177.87(18) . 2_545 ?
O2 Li4 O3 93.9(2) 4_545 2_545 ?
O2 Li4 O3 86.3(2) 3_445 2_545 ?
O3 Li4 O3 83.8(3) 1_545 2_545 ?
O1 Li4 Li1 134.9(3) 2 . ?
O1 Li4 Li1 48.0(3) . . ?
O2 Li4 Li1 87.0(2) 4_545 . ?
O2 Li4 Li1 93.0(2) 3_445 . ?
O3 Li4 Li1 46.7(3) 1_545 . ?
O3 Li4 Li1 130.4(3) 2_545 . ?
O1 Li4 Li1 48.0(3) 2 2 ?
O1 Li4 Li1 134.9(3) . 2 ?
O2 Li4 Li1 93.0(2) 4_545 2 ?
O2 Li4 Li1 87.0(2) 3_445 2 ?
O3 Li4 Li1 130.4(3) 1_545 2 ?
O3 Li4 Li1 46.7(3) 2_545 2 ?
Li1 Li4 Li1 177.1(5) . 2 ?
O1 Li4 Li2 48.27(15) 2 . ?
O1 Li4 Li2 87.33(16) . . ?
O2 Li4 Li2 46.96(13) 4_545 . ?
O2 Li4 Li2 132.82(16) 3_445 . ?
O3 Li4 Li2 132.95(15) 1_545 . ?
O3 Li4 Li2 92.95(14) 2_545 . ?
Li1 Li4 Li2 121.2(2) . . ?
Li1 Li4 Li2 60.4(2) 2 . ?
O1 Li4 Li2 87.33(16) 2 2 ?
O1 Li4 Li2 48.27(15) . 2 ?
O2 Li4 Li2 132.82(16) 4_545 2 ?
O2 Li4 Li2 46.96(13) 3_445 2 ?
O3 Li4 Li2 92.95(14) 1_545 2 ?
O3 Li4 Li2 132.95(15) 2_545 2 ?
Li1 Li4 Li2 60.4(2) . 2 ?
Li1 Li4 Li2 121.2(2) 2 2 ?
Li2 Li4 Li2 121.04(11) . 2 ?
O1 Li4 Li1 132.4(3) 2 5 ?
O1 Li4 Li1 92.7(2) . 5 ?
O2 Li4 Li1 132.3(3) 4_545 5 ?
O2 Li4 Li1 47.9(3) 3_445 5 ?
O3 Li4 Li1 46.4(3) 1_545 5 ?
O3 Li4 Li1 87.0(3) 2_545 5 ?
Li1 Li4 Li1 58.4(4) . 5 ?
Li1 Li4 Li1 119.9(3) 2 5 ?
Li2 Li4 Li1 179.3(2) . 5 ?
Li2 Li4 Li1 59.4(2) 2 5 ?
O1 Li4 Li1 92.7(2) 2 6_556 ?
O1 Li4 Li1 132.4(3) . 6_556 ?
O2 Li4 Li1 47.9(3) 4_545 6_556 ?
O2 Li4 Li1 132.3(3) 3_445 6_556 ?
O3 Li4 Li1 87.0(3) 1_545 6_556 ?
O3 Li4 Li1 46.4(3) 2_545 6_556 ?
Li1 Li4 Li1 119.9(3) . 6_556 ?
Li1 Li4 Li1 58.4(4) 2 6_556 ?
Li2 Li4 Li1 59.4(2) . 6_556 ?
Li2 Li4 Li1 179.3(2) 2 6_556 ?
Li1 Li4 Li1 120.2(4) 5 6_556 ?
O2 Cr2 O2 84.5(3) . 2 ?
O2 Cr2 O1 93.7(2) . . ?
O2 Cr2 O1 176.96(17) 2 . ?
O2 Cr2 O1 176.96(17) . 2 ?
O2 Cr2 O1 93.7(2) 2 2 ?
O1 Cr2 O1 88.3(3) . 2 ?
O2 Cr2 O3 93.5(2) . 3_445 ?
O2 Cr2 O3 89.7(2) 2 3_445 ?
O1 Cr2 O3 92.8(2) . 3_445 ?
O1 Cr2 O3 84.0(2) 2 3_445 ?
O2 Cr2 O3 89.7(2) . 4_545 ?
O2 Cr2 O3 93.5(2) 2 4_545 ?
O1 Cr2 O3 84.0(2) . 4_545 ?
O1 Cr2 O3 92.8(2) 2 4_545 ?
O3 Cr2 O3 175.6(2) 3_445 4_545 ?
O2 Cr2 Li1 88.4(3) . 4 ?
O2 Cr2 Li1 46.8(2) 2 4 ?
O1 Cr2 Li1 130.9(3) . 4 ?
O1 Cr2 Li1 92.1(3) 2 4 ?
O3 Cr2 Li1 136.1(2) 3_445 4 ?
O3 Cr2 Li1 46.9(2) 4_545 4 ?
O2 Cr2 Li1 46.8(2) . 3_455 ?
O2 Cr2 Li1 88.4(3) 2 3_455 ?
O1 Cr2 Li1 92.1(3) . 3_455 ?
O1 Cr2 Li1 130.9(3) 2 3_455 ?
O3 Cr2 Li1 46.9(2) 3_445 3_455 ?
O3 Cr2 Li1 136.1(2) 4_545 3_455 ?
Li1 Cr2 Li1 122.4(4) 4 3_455 ?
O2 Cr2 Sb1 42.26(13) . . ?
O2 Cr2 Sb1 42.26(14) 2 . ?
O1 Cr2 Sb1 135.86(13) . . ?
O1 Cr2 Sb1 135.86(13) 2 . ?
O3 Cr2 Sb1 92.18(12) 3_445 . ?
O3 Cr2 Sb1 92.18(12) 4_545 . ?
Li1 Cr2 Sb1 61.2(2) 4 . ?
Li1 Cr2 Sb1 61.2(2) 3_455 . ?
O2 Cr2 Li4 137.74(13) . . ?
O2 Cr2 Li4 137.74(14) 2 . ?
O1 Cr2 Li4 44.14(13) . . ?
O1 Cr2 Li4 44.14(13) 2 . ?
O3 Cr2 Li4 87.82(12) 3_445 . ?
O3 Cr2 Li4 87.82(12) 4_545 . ?
Li1 Cr2 Li4 118.8(2) 4 . ?
Li1 Cr2 Li4 118.8(2) 3_455 . ?
Sb1 Cr2 Li4 180 . . ?
Li3 O1 Sb1 0.00(4) 3_545 3_545 ?
Li3 O1 Cr2 94.8(2) 3_545 . ?
Sb1 O1 Cr2 94.8(2) 3_545 . ?
Li3 O1 Li4 93.5(2) 3_545 . ?
Sb1 O1 Li4 93.5(2) 3_545 . ?
Cr2 O1 Li4 92.2(2) . . ?
Li3 O1 Li1 91.4(3) 3_545 7 ?
Sb1 O1 Li1 91.4(3) 3_545 7 ?
Cr2 O1 Li1 90.4(3) . 7 ?
Li4 O1 Li1 174.3(4) . 7 ?
Li3 O1 Li1 91.3(3) 3_545 . ?
Sb1 O1 Li1 91.3(3) 3_545 . ?
Cr2 O1 Li1 173.9(4) . . ?
Li4 O1 Li1 87.6(3) . . ?
Li1 O1 Li1 89.3(5) 7 . ?
Li3 O1 Li2 176.1(3) 3_545 2 ?
Sb1 O1 Li2 176.1(3) 3_545 2 ?
Cr2 O1 Li2 88.95(19) . 2 ?
Li4 O1 Li2 87.43(19) . 2 ?
Li1 O1 Li2 87.5(3) 7 2 ?
Li1 O1 Li2 84.9(3) . 2 ?
Sb1 O2 Cr2 94.7(2) . . ?
Sb1 O2 Cr1 92.9(2) . 3 ?
Cr2 O2 Cr1 92.6(2) . 3 ?
Sb1 O2 Li4 92.9(2) . 3 ?
Cr2 O2 Li4 92.6(2) . 3 ?
Cr1 O2 Li4 0.00(17) 3 3 ?
Sb1 O2 Li1 92.9(4) . 3_455 ?
Cr2 O2 Li1 89.7(3) . 3_455 ?
Cr1 O2 Li1 173.6(4) 3 3_455 ?
Li4 O2 Li1 173.6(4) 3 3_455 ?
Sb1 O2 Li2 90.96(16) . 4 ?
Cr2 O2 Li2 174.3(3) . 4 ?
Cr1 O2 Li2 87.98(19) 3 4 ?
Li4 O2 Li2 87.98(19) 3 4 ?
Li1 O2 Li2 89.1(3) 3_455 4 ?
Sb1 O2 Li1 175.4(4) . 7 ?
Cr2 O2 Li1 89.9(3) . 7 ?
Cr1 O2 Li1 87.2(3) 3 7 ?
Li4 O2 Li1 87.2(3) 3 7 ?
Li1 O2 Li1 86.8(5) 3_455 7 ?
Li2 O2 Li1 84.5(3) 4 7 ?
Sb1 O3 Sb5 94.7(2) . 3 ?
Sb1 O3 Li5 94.7(2) . 3 ?
Sb5 O3 Li5 0 3 3 ?
Sb1 O3 Cr2 94.7(2) . 3 ?
Sb5 O3 Cr2 0 3 3 ?
Li5 O3 Cr2 0 3 3 ?
Sb1 O3 Cr1 93.3(2) . 1_565 ?
Sb5 O3 Cr1 91.37(19) 3 1_565 ?
Li5 O3 Cr1 91.37(19) 3 1_565 ?
Cr2 O3 Cr1 91.37(19) 3 1_565 ?
Sb1 O3 Li4 93.3(2) . 1_565 ?
Sb5 O3 Li4 91.37(19) 3 1_565 ?
Li5 O3 Li4 91.37(19) 3 1_565 ?
Cr2 O3 Li4 91.37(19) 3 1_565 ?
Cr1 O3 Li4 0 1_565 1_565 ?
Sb1 O3 Li2 92.11(17) . 4 ?
Sb5 O3 Li2 91.4(2) 3 4 ?
Li5 O3 Li2 91.4(2) 3 4 ?
Cr2 O3 Li2 91.4(2) 3 4 ?
Cr1 O3 Li2 173.7(3) 1_565 4 ?
Li4 O3 Li2 173.7(3) 1_565 4 ?
Sb1 O3 Li1 91.9(3) . 5_565 ?
Sb5 O3 Li1 173.4(4) 3 5_565 ?
Li5 O3 Li1 173.4(4) 3 5_565 ?
Cr2 O3 Li1 173.4(4) 3 5_565 ?
Cr1 O3 Li1 88.2(4) 1_565 5_565 ?
Li4 O3 Li1 88.2(4) 1_565 5_565 ?
Li2 O3 Li1 88.4(4) 4 5_565 ?
Sb1 O3 Li1 176.1(4) . 1_565 ?
Sb5 O3 Li1 89.0(3) 3 1_565 ?
Li5 O3 Li1 89.0(3) 3 1_565 ?
Cr2 O3 Li1 89.0(3) 3 1_565 ?
Cr1 O3 Li1 87.6(3) 1_565 1_565 ?
Li4 O3 Li1 87.6(3) 1_565 1_565 ?
Li2 O3 Li1 86.8(4) 4 1_565 ?
Li1 O3 Li1 84.4(5) 5_565 1_565 ?

# The following lines are used to test the character set of files sent by
# network email or other means. They are not part of the CIF data set
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./

# END of CIF
_database_code_depnum_ccdc_archive 'CCDC 980559'
